Presentation on theme: "Franklyn B.S.121050xx Febianda Primatama12506004 M. Lukman 12506016 Yoga Baskoro Adi12506023 Anita C.S12506029 Program Studi Teknik Metalurgi Fakultas."— Presentation transcript:
Franklyn B.S xx Febianda Primatama M. Lukman Yoga Baskoro Adi Anita C.S Program Studi Teknik Metalurgi Fakultas Teknik Pertambangan dan Perminyakan Institut Teknologi Bandung 2009
Alloy 304L (UNS S30403) stainless steel plate is a variation of the 18% chromium – 8% nickel austenitic alloy, the most familiar and most frequently used alloy in the stainless steel family. This alloy may be considered for a wide variety of applications and exhibits good corrosion resistance, ease of fabrication, excellent formability, and high strength with low weight.
Resistance to corrosion Prevention of product contamination Resistance to oxidation Ease of fabrication Excellent formability Beauty of appearance Ease of cleaning High strength with low weight Good strength and toughness at cryogenic temperatures Ready availability of a wide range of product forms
Element Percentage by Weight Maximum Unless Range is Specified L304H Carbon Manganese2.00 Phosphorus0.045 Sulfur0.030 Silicon0.75 Chromium Nickel Nitrogen0.10
% Nitric Acid Temperature ° F (°C) Corrosion Rate Mils/Yr (mm/a) (149)5.0 (0.13) (149)10.1 (0.25) (149)17.0 (0.43) General Corrosion 304L provide useful resistance to corrosion on a wide range of moderately oxidizing to moderately reducing environments.
Intergranular Corrosion Tests ASTM A262 Evaluation Test Corrosion Rate, Mils/Yr (mm/a) L Practice E Base Metal Welded No Fissures on Bend Some Fissures on Weld (unaccepta ble)No Fissures Practice A Base Metal Welded Step Structure Ditched (unaccepta ble)Step Structure Intergranular Corrosion Exposure of the 18-8 austenitic stainless steels to temperatures in the 800°F to 1500°F (427°C to 816°C) range may cause precipitation of chromium carbides in grain boundaries. Such steels are "sensitized" and subject to intergranular corrosion when exposed to aggressive environments. The carbon content of Alloy 304 may allow sensitization to occur from thermal conditions experienced by autogenous welds and heat-affected zones of welds. For this reason, the low carbon Alloy 304L is preferred for applications in which the material is put into service in the as-welded condition. Low carbon content extends the time necessary to precipitate a harmful level of chromium carbides but does not eliminate the precipitation reaction for material held for long times in the precipitation temperature range.
Pitting /Crevise Corrosion The 18-8 alloys have been used very successfully in fresh waters containing low levels of chloride ion. Generally, 100 ppm chloride is considered to be the limit for the 18-8 alloys, particularly if crevices are present. Higher levels of chloride might cause crevice corrosion and pitting. For the more severe conditions of higher chloride levels, lower pH, and/or higher temperatures, alloys with higher molybdenum content such as Alloy 316 should be considered. The 18-8 alloys are not recommended for exposure to marine environments.
Density: lb/in3 (7.90 g/cm3) Modulus of Elasticity in Tension: 29 x 10 6 psi (200 GPa) Linear Coefficient of Thermal Expansion: Temperature RangeCoefficients °F°Cin/in/°Fcm/cm/°C x x x x 10 -6
Thermal Conductivity: Temperature Range Btu/hr/ft /°F W/m /K °F°C Specific Heat: °F°CBtu/lb/°F J/kg/ K Magnetic Permeability: Percent Cold Work Magnetic Permeability L
Room Temperature Mechanical Properties Property Minimum Mechanical Properties Required by ASTM A240 & ASME SA L304H 0.2% Offset Yield Strength, psi MPa30, , , Ultimate Tensile Strength, psi MPa 75, , , Percent Elongation in 2 in. or 51 mm40.0 Hardness, Max., Brinell R B Impact Resistance Temperature Charpy V-Notch Energy Absorbed °F°C Foot - pounds Joules
Test Temperature 0.2% Yield Strength Tensile Strength Elongation °F°Cpsi(MPa)psiMPa Percent in 2" or 51mm , , , , , , , , , , , , , , , , Low and Elevated Temperature Properties Typical short time tensile property data for low and elevated temperatures are shown below. At temperatures of 1000°F (538°C) or higher, creep and stress rupture become considerations. Typical creep and stress rupture data are also shown below.
The fatigue strength or endurance limit is the maximum stress below which material is unlikely to fail in 10 million cycles in air environment. The fatigue strength for austenitic stainless steels, as a group, is typically about 35 percent of the tensile strength. Substantial variability in service results is experienced since additional variables influence fatigue strength. As examples – increased smoothness of surface improves strength, increased corrosivity of service environment decreases strength. Fatigue Strength
The austenitic stainless steels are heat treated to remove the effects of cold forming or to dissolve precipitated chromium carbides. The surest heat treatment to accomplish both requirements is the solution anneal which is conducted in the 1850°F to 2050°F range (1010°C to 1121°C). Cooling from the anneal temperature should be at sufficiently high rates through °F (816°C - 427°C) to avoid reprecipitation of chromium carbides. These materials cannot be hardened by heat treatment.
Two important considerations in producing weld joints in the austenitic stainless steels are: 1) preservation of corrosion resistance, and 2) avoidance of cracking. The higher the carbon level of the material being welded, the greater the likelihood that the welding thermal cycle will result in the chromium carbide precipitation which is detrimental to corrosion resistance. To provide material at the best level of corrosion resistance, low carbon material (Alloy 304L) should be used for material put in service in the welded condition. Alternately, full annealing dissolves the chromium carbide and restores a high level of corrosion resistance to the standard carbon content materials. Alloy 309 (23% Cr – 13.5% Ni) or nickel-base filler metals are used in joining the 18-8 austenitic alloys to carbon steel.
Sanitary Dairy and Food processing Heat exchangers Evaporators Feedwater heaters Architecture Plant for chemical, petrochemical, mineral processing and other industries.